A greatly increased colloidal stability of the IONPs and functionalization of the amine group were expected from this process. Furthermore, when the available amine-functionalized CLNPs were observed by RITC conjugation, they attempted to conjugate two different biological molecules. TEM image of IONP (a) before ligand exchange and (b) after ligand exchange. c) DLS data for IONPs after the ligand exchange and purification step.
Camera image of stability of (a) IONPs-PEG (c) IONPs-AA and (e) CLNPs in wide range of pHs. Camera image of stability of (a) IONPs-PEG (c) IONPs-AA and (e) CLNPs in various concentrations of NaCl solutions. FT-IR data of CLNPs (black) and CLNPs-Man (red) to confirm the mannose-conjugated CLNPs. a) DLS data of after folic acid conjugated to CLNPs (b) UV-Vis absorption analysis to confirm folic acid conjugation.
Microscopy image of Prussian blue stained HeLa cell treated with (a) 200 uM and (c) 500 uM CLNPs. Scheme of CLNPs-Man incubated with Con A led to the formation of aggregates, resulting in shorter T2 relaxation time and consequently a darkened MRI image.
- General properties of iron oxide nanoparticles (IONPs)
- Surface modification of IONPs
- Colloidal stability of IONPs
- IONPs for bio-applications
To meet this requirement, the surface modification process of IONPs is necessary, and this surface modification field was researched for many decades. For example, Jon et al.30 reported thermally crosslinked superparamagnetic iron oxide nanoparticles (TCL-SPION), which crosslinked with thermal reaction of Si–OH-containing copolymer as opposed to chemical crosslinking system30. Very stable polymer coating was performed, PEG-silane copolymer was crosslinked as hydrolysis of silane groups (-Si(OH)3) by simple heat treatment.
The other approach for cross-linking was reported by Kim et al. They developed cross-linked polymer nano-assemblies by cross-linking poly(succinimide) (PSI) with hexamethylenedimaine (HMD) linker (Figure 3b), and they were successfully prepared to form a show strong potential for bioapplications. Scheme of (a) poly(TMSMA-r-PEGMA-r-NAS) (top), carboxyl TCL-SPION showing cross-linking between polymer layers after heat treatment (bottom)30. b) cross-linked magnetic nanoparticles after cross-linking between PSI-g-PEG-C12 layers with hexamethylenediamine (HMD)31. The bioapplications of IONPs include well-known contrast agents for magnetic resonance imaging (MRI)33-35, cancer cell targeting36-37 and magnetoresponsive therapy38-39 (Figure 1)1.
IONPs are the most suitable substances that can be alternative MRI contrast agents due to their high biocompatibility. Compact and cross-linked nanoparticles: nanoplatform for highly stable, versatile conjugation and its bioapplication.
Compact and cross-linked nanoparticles: nano-platform for highly stable, versatile
To confirm cross-linked nanoparticles, XPS spectra were used and visualization of CLNPs was attempted by TEM analysis with negative staining method. Add DMF dissolved maleimide propionic acid as 1 equivalent ratio to the amine group of CLNPs. To conjugate folic acid to amine-functionalized CLNPs, prepare 1 equivalent ratio of folic acid to the concentration of CLNPs in 1xPBS (pH 7.4) solution.
After crosslinking reaction, hydrodynamic diameter (HD) of CLNPs was measured by DLS to confirm that the size of CLNPs was maintained after reaction. Also, analysis of zeta potential of CLNPs was required to compare the extent of crosslinking reaction with different concentrations of diamines. This suggests that some of the ligands bound to the surface of CLNPs may be retained.
In this study, several verification tools for colloidal stability were proposed and the stability of CLNPs was confirmed. To overcome these unstable conditions, CLNPs retained their size in NaCl at each concentration, proving the stability of CLNPs (Fig. 15c). These results suggest that bioapplication without any aggregation is possible even with application of CLNPs to the azide–alkyne conjugation method.
These different tools were used to confirm the stability of the particles and the possibility of further reaction of the CLNPs. In previous experiments, after amine functionalization of CLNPs was confirmed by RITC conjugation (figure 9). After all processes and redispersion in 1xPBS buffer, the size of CLNPs-Man was compact without any aggregates (figure 17).
CLNPs-Man binding was analyzed by high-resolution magic-angle spinning (HR-MAS) (figure 18). After the conjugation of folic acid with the CLNPs process, the size of the CLNPs-FA appeared to maintain the stable HD size of ~24 nm without any aggregation (Figure 20a). Through these results, mannose immobilized on CLNPs retain their biorecognition specificity, indeed, the application of in vitro and in vivo targeting powers of CLNPs was confirmed.
Materials & Experimental methods
- Instrumental and analysis
- Synthesis of iron-oleate complex
- Synthesis of iron oxide nanoparticles
- Synthesis of ligand by RAFT polymerization
- Ligand exchange of 12 nm IONPs
- Cross linking of IONPs (CLNPs)
- Conjugation of rhodamine B isocyanate to CLNPs
- Synthesis of maleimide propionic acid
- Conjugation of mannose
- Conjugation of folic acid
- MR relaxivity
- Cell culture
- Prussian blue staining
Results & Discussion
- Synthesis of ligand & water dispersible IONPs
- Cross linking with various diamines
- Confirmation of cross linked IONPs (CLNPs)
- Various stability test of CLNPs
- Multifunctional conjugation of CLNPs
- Specific targeting test by MR relaxivity
- In vitro test with folic acid conjugated CLNPs
This result is due to the reduced stability of the IONPs due to the interaction between the fast protein liquid chromatography (FPLC) column during the purification process when the long polymer is used (Figure 5a). As a result, it was found that the stability of the particles decreases as the ratio of carboxyl groups decreases (Figure 5b). Finally, the stability of IONPs was confirmed by increasing the addition ratio of anchor group, DMA to 30, 40 and 50%.
For further comparison of these results, we confirmed the stability of each ligand-exchanged IONPs in a hard 'click' chemistry condition (Figure 5d). Schematic of the optimized ligand for ligand exchange of Fe3O4 iron oxide nanoparticles (IONPs) in this study. To overcome this limitation, we improved the stability of ligand-exchanged IONPs by cross-linking the surface ligands through EDC coupling with diamine (Scheme 3).
As a result, the zeta potential value of CLNPs with hexamethylenediamine was found to be the least neutral mV because the carboxyl group and both amines were well coupled, meaning that the cross-linking with HDM in this condition was well performed. This can be interpreted as both amines of HDM were well conjugated to the carboxyl group of the surface. These results ensured diamine cross-linking that improves the stability of the IONPs and allowed amine functionalization to be achieved at the same time.
Hydrodynamic diameter (nm) and zeta potential (mV) values measured by DLS, which used different diamines for cross-linking. This result indicates that HDM was involved in the cross-linking of IONPs by EDC by binding to the carboxylic acid of the surface of IONPs. of HDM to compare the N1 and C1 energy binding peak analyzed by XPS spectra. The biggest advantage of cross-linking is that the stability of the IONPs is maximized.
Unlike the other IONPs, CLNPs remained stable over the entire pH range for one week because the cross-linking reaction ensured the stability of IONPs (Fig. 14c). First, one of the monosaccharide types, mannose (Man), was conjugated to CLNPs to confirm amine functionalization. To separate the signal for more detailed analysis, the signal 3.65 ppm indicates the organic ligand of CLNPs.
With this result, CLNP-FAs were successfully designed and it shows that CLNPs are very stable in all other reactions and also the amine groups of CLNPs are accessible for bioconjugation.
Ling, D.; Lee, N.; Hyeon, T., Chemical Synthesis and Assembly of Uniformly Sized Iron Oxide Nanoparticles for Medical Applications. H.; Hyeon, T., Large-scale synthesis of uniform and ultrasmall iron oxide nanoparticles for high-resolution T1 magnetic resonance imaging contrast agents. Lee, N.; Hyeon, T., Planned Synthesis of Uniformly Sized Iron Oxide Nanoparticles for Effective Magnetic Resonance Imaging Contrast Agents.
N.; Sanyal, R.; Sanyal, A., Modular fabrication of polymer brush-coated magnetic nanoparticles: engineering the interface for targeted cellular imaging. C.; Mattoussi, H., Multidentate Catechol-based Polyethylene Glycol Oligomers Offer Enhanced Stability and Biocompatibility with Iron Oxide Nanoparticles. T; Weissleder, R., Tat peptide-derivatized magnetic nanoparticles enable in vivo tracking and recovery of progenitor cells.
N.; Jon, S., Antibiofouling amphiphilic polymer coated superparamagnetic iron oxide nanoparticles: synthesis, characterization, and use in cancer imaging in vivo. Y.; Kang, H.-W.; Jon, S., Thermally cross-linked superparamagnetic iron oxide nanoparticles: synthesis and application as a dual imaging probe for cancer in vivo. Poselt, E.; Kloust, H.; Tromsdorf, U.; Janschel, M.; Hahn, C.; Masslo, C.; Weller, H., Relaxivity optimization of a pegylated iron oxide-based negative magnetic resonance contrast agent for T2-weighted spin-echo imaging.
A.; Yang, L.; Mao, H., Enhanced permeability and retention effect driven delivery by ultrafine iron oxide nanoparticles with T1-T2 switchable magnetic resonance imaging contrast. Espinosa, A.; Di Corato, R.; Kolosnjaj-Tabi, J.; Flaud, P.; Pellegrino, T.; Wilhelm, C., Duality of iron oxide nanoparticles in cancer therapy: enhancement of heating efficiency by magnetic hyperthermia and photothermal bimodal treatment. Li, L.; Jiang, W.; Luo, K.; Song, H.; Lan, F.; Wu, Y.; Gu, Z., Superparamagnetic iron oxide nanoparticles as MRI contrast agents for noninvasive stem cell labeling and tracking.
Sonvico, F.; Mornet, S.; Vasseur, S.; Dubernet, C.; Jaillard, D.; Degrouard, J.; Hoebeke, J.; Duguet, E.; Colombo, P.; Couvreur, P., Folate-conjugated iron oxide nanoparticles for solid tumor targeting as potential specific magnetic hyperthermia mediators: synthesis, physicochemical characterization and in vitro experiments. Yang, Y.; Li, Y.; Lin, Q.; Bao, C.; Zhu, L., In Situ Phototriggered Disulfide-Cross-Link Nanoparticles for Drug Delivery. A.; Mohindra, P.; Tong, S.; Bao, G., Multifunctional superparamagnetic iron oxide nanoparticles for combined chemotherapy and hyperthermia cancer treatment.